1 Page 1 of 12 Unit Display: English Print Now Custom 455 Stainless Datasheet Add to My Materials UNS Number S45500 Identification Type Analysis Carbon 0.05 % Manganese 0.50 % Phosphorus % Sulfur % Silicon 0.50 % Chromium to % Nickel 7.50 to 9.50 % Molybdenum 0.50 % Copper 1.50 to 2.50 % Titanium 0.80 to 1.40 % Columbium + Tantalum 0.10 to 0.50 % Iron to % General Information Description Recognizing the need for high-strength alloys with good corrosion resistance to atmospheric environments, the Carpenter Research Laboratory developed Custom 455 stainless, a martensitic age-hardenable stainless steel. This alloy is relatively soft and formable in the annealed condition. A single-step aging treatment develops exceptionally high yield strength with good ductility and toughness. This stainless can be machined in the annealed condition, and welded in much the same manner as other precipitation hardenable stainless steels. Because of its low work-hardening rate, it can be extensively cold formed. The dimensional change during hardening is only about in/in, which permits close-tolerance finish machining in the annealed state. Custom 455 stainless represents a significant advancement in the area of precipitation hardening stainless steels. It should be considered where simplicity of heat treatment, ease of fabrication, high strength and corrosion resistance are required in combination. Selection Because of the unique combination of high strength and corrosion resistance of Custom 455 stainless there are a few other alloys available for consideration. Carpenter 13-8 stainless can be considered where good transverse toughness and ductility are necessary in large sections. Elevated Temperature Use Custom 455 stainless has displayed excellent resistance to oxidation up to approximately 1100 F (593 C). Long-term exposure to elevated temperatures can result in reduced toughness in precipitation hardenable stainless steels. The reduction in toughness can be minimized in some cases by using higher aging temperatures. Short exposures to elevated temperatures can be considered, provided the maximum temperature is at least 50 F (28 C) less than the aging temperature. Corrosion Resistance Custom 455 stainless resists staining in normal air atmospheres, and shows no corrosion in fresh water. Tests in 5% salt spray at 95 F (35 C) and in 5% ferric chloride at room temperature have demonstrated good resistance to pitting and rusting. Laboratory tests in a variety of mild chemical environments have shown that the level of general corrosion resistance is superior to that of the 12% chromium steels (Type 410) and approaches that of the 17% chromium steels (Type 430). In most tests there was no significant effect of aging temperature on corrosion resistance. Hydrogen embrittlement tests in 5% acetic acid saturated with H2S at room temperature show the same degree of susceptibility as other high-strength martensitic stainless steels. All high-strength steels are subject to stress corrosion under certain stress conditions and in certain environments. Numerous severe tests have been conducted to evaluate the behavior of Custom 455 stainless in different environments and to determine the effect of aging temperature on resistance to stress-corrosion cracking. These tests include U-bend specimens, direct tension specimens, C-rings and precracked cantilever beam specimens. Environments have included marine atmospheres, 20% salt spray, and 3-1/2% sodium chloride solutions. All tests have shown that Custom 455 stainless has inherently good resistance to stress-corrosion cracking, and that this resistance improves markedly as aging temperature is increased. For optimum corrosion resistance, surfaces must be free of scale, lubricants, foreign particles, and coatings applied for drawing and heading. After fabrication of parts, cleaning and/or passivation should be considered. Important Note:The following 4-level rating scale is intended for comparative purposes only. Corrosion testing
2 Page 2 of 12 is recommended; factors which affect corrosion resistance include temperature, concentration, ph, impurities, aeration, velocity, crevices, deposits, metallurgical condition, stress, surface finish and dissimilar metal contact. Nitric Acid Moderate Sulfuric Acid Restricted Phosphoric Acid Restricted Acetic Acid Restricted Sodium Hydroxide Moderate Salt Spray (NaCl) Good Sea Water Restricted Humidity Excellent Properties Physical Properties Specific Gravity Annealed 7.76 Condition H Condition H Condition H Condition H Condition H Density Annealed lb/in³ Condition H lb/in³ Condition H lb/in³ Condition H lb/in³ Condition H lb/in³ Condition H lb/in³ Mean Coefficient of Thermal Expansion 72 F, 200 F 72 F, 300 F 72 F, 500 F 72 F, 700 F 72 F, 900 F 5.90 x 10-6 in/in/ F 6.03 x 10-6 in/in/ F 6.20 x 10-6 in/in/ F 6.45 x 10-6 in/in/ F 6.68 x 10-6 in/in/ F Thermal Conductivity 212 F BTU-in/hr/ft²/ F 392 F BTU-in/hr/ft²/ F 572 F BTU-in/hr/ft²/ F 752 F BTU-in/hr/ft²/ F 932 F BTU-in/hr/ft²/ F
3 Page 3 of 12 Poisson's Ratio Modulus of Elasticity (E) x 10 3 ksi Modulus of Rigidity (G) x 10 3 ksi Electrical Resistivity 70.0 F, Condition A ohm-cir-mil/ft 70.0 F, Condition H ohm-cir-mil/ft Typical Mechanical Properties
4 Page 4 of 12
5 Page 5 of 12
6 Page 6 of 12
7 Page 7 of 12 Toughness Fracture toughness is the resistance of a material to abrupt, brittle failure at stresses below its yield strength when various stress concentrators are present. It is described by a stress intensity parameter K. Custom 455 stainless has good fracture toughness after various aging treatments. Heat Treatment Solution Treatment Condition A (Solution Treated or Annealed): Heat to 1500/1550 (816/843 C), and cool rapidly. Water quenching is preferred for small sections. Custom 455 stainless will normally be supplied from the mill in the annealed condition, ready for the one-step hardening treatment. Age Condition H 900, H 950, H 1000, H 1050 (Precipitation or Age Hardened): The high strength levels of Carpenter Custom 455 stainless are derived from a simple precipitation-hardening treatment consisting of heating to a selected temperature between 900/1050 F (482/566 C), holding for four hours and air cooling.
8 Page 8 of 12 Hot Working Workability Custom 455 stainless is easily forged within the temperature range of 1650/2300 F (899/1260 C). For optimum mechanical properties, material to be forged should be heated uniformly to 1900/2100 F (1038/1149 C) and soaked at heat; finishing temperature should be within the range of 1500/1700 F (816/927 C) to obtain an optimum grain size and properties after heat treating. Cool forgings in air to room temperature and anneal. Cold Working Cold working is readily performed despite the fact that Custom 455 stainless is martensitic in the annealed condition, and has a hardness of Rockwell C 30/35. Deep drawing or stretching operations will require intermediate anneals because the elongation tends to be localized. For other cold-forming operations such as cold drawing and cold rolling, the work-hardening rate in the annealed condition is extremely low allowing considerable cold working without intermediate annealing. Cold-heading and warm-heading operations are also easily performed. Cold working prior to aging results in even higher tensile and yield strengths in the hardened condition. Spring Properties: Wire in the annealed or lightly drawn condition and annealed strip can be aged for 2 to 4 hours at 900 F (482 C) to achieve a tensile strength in excess of 250 ksi (1742 MPa). As such, Custom 455 stainless can be used in relatively large diameters and thicknesses and still have good spring characteristics. This greatly expands the range of sizes of corrosion-resistant springs available to designer. Custom 455 stainless can also be extensively cold worked prior to aging to achieve even higher levels of strength. Extensive cold working reduces the aging time required to reach maximum mechanical properties. Therefore, colddrawn spring wire and cold-rolled strip in Condition C need only be aged for ½ hour at 850 F (454 C).
9 Page 9 of 12 Machinability Custom 455 stainless has been machined successfully using the same practices required for other high-strength alloys; i.e., rigid tool and work supports, slower speeds, positive cuts and adequate amounts of coolant. The machining characteristics of Custom 455 stainless are similar to those of the nickel maraging steels. Following are typical feeds and speeds for Custom 455 stainless.
10 Page 10 of 12
11 Page 11 of 12 Additional Machinability Notes Figures used for all metal removal operations covered are starting points. On certain work, the nature of the part may require adjustment of speeds and feeds. Each job has to be developed for best production results with optimum tool life. Speeds or feeds should be increased or decreased in small steps. Weldability Custom 455 stainless can be satisfactorily welded by the shielded fusion and resistance welding processes. Oxyacetylene welding is not recommended, since carbon pickup in the weld may occur. Preheating is not required to prevent cracking during the welding of this alloy. Normally, welding in the solution-annealed condition is satisfactory; however, where high welding stresses are anticipated, it may be advantageous to weld in the overaged [aged at 1150 F (621 C)] condition. If welded in the solution-annealed condition, the alloy can be directly aged to the desired strength level after welding. However, the optimum combination of strength, ductility and corrosion resistance is obtained by solution annealing the welded part before aging. If welded in the overaged condition, the part should be solution annealed before aging. Descaling (Cleaning) Other Information Descaling following forging and annealing can be accomplished by acid cleaning or grit blasting. The acid treatment consists of 2 minutes in 50% by volume muriatic acid at 180 F (82 C), followed by 4 minutes in a mixture of 15% by volume nitric acid, plus 3% by volume hydrofluoric acid at room temperature. Repeat cleaning procedure as necessary but decrease the times by 50% (i.e., 1 and 2 minutes, respectively).
12 Page 12 of 12 The heat tint from aging can be removed by polishing, vapor blasting or pickling 4 to 6 minutes in a mixture of 15% by volume nitric acid, plus 3% by volume hydrofluoric acid, followed by a water rinse. Repeat the acid cleaning procedure if necessary, but decrease the time by 2 to 3 minutes. Desmut in 20% by volume nitric acid at room temperature. After acid cleaning, bake 1 to 3 hours at 300/350 F (149/177 C) to remove hydrogen. Applicable Specifications AMS 5617 AMS 5860 (Strip) ASME SA564 ASTM A564 (XM-16) ASTM A693 (XM-16) Forms Manufactured Bar-Flats Bar-Rounds Bar-Shapes Bar-Squares Billet Strip Wire Technical Articles A Designer's Manual On Specialty Alloys For Critical Automotive Components A Guide to Etching Specialty Alloys for Microstructural Evaluation Advanced Stainless Offers High Strength, Toughness and Corrosion Resistance Wherever Needed Alloy Selection for Cold Forming (Part I) Alloy Selection for Cold Forming (Part II) How to Passivate Stainless Steel Parts How to Select the Right Stainless Steel or High Temperature Alloy for Heading Improved Stainless Steels for Medical Instrument Tubing New Ideas for Machining Austenitic Stainless Steels New Ph Stainless Combines High Strength, Fracture Toughness and Corrosion Resistance New Requirements for Ferrous-Base Aerospace Alloys New Stainless Steel for Instruments Combines High Strength and Toughness Passivating and Electropolishing Stainless Steel Parts Selecting New Stainless Steels for Unique Applications Selecting Stainless Steels for Valves Selection of High Strength Stainless Steels for Aerospace, Military and Other Critical Applications Specialty Alloys And Titanium Shapes To Consider For Latest Medical Materials Requirements Steels for Strength and Machinability Unique Properties Required of Alloys for the Medical and Dental Products Industry Disclaimer: The information and data presented herein are typical or average values and are not a guarantee of maximum or minimum values. Applications specifically suggested for material described herein are made solely for the purpose of illustration to enable the reader to make his/her own evaluation and are not intended as warranties, either express or implied, of fitness for these or other purposes. There is no representation that the recipient of this literature will receive updated editions as they become available. Unless otherwise specified, registered trademarks are property of CRS Holdings Inc., a subsidiary of Carpenter Technology Corporation. Copyright 2009 CRS Holdings Inc. All rights reserved. Edition Date: 6/9/06